O R I G I N A L P A P E R
Decomposition of Urea in the SCR Process: Combination of DFT
Calculations and Experimental Results on the Catalytic
Hydrolysis of Isocyanic Acid on TiO2
Izabela CzekajÆ Oliver Kro¨cher
Published online: 10 July 2009
Ó Springer Science+Business Media, LLC 2009
Abstract In selective catalytic reduction (SCR) systems for diesel vehicles the injected urea solution decomposes to ammonia and isocyanic acid (HNCO), which reacts with water to another ammonia molecule and carbon dioxide over the SCR catalyst or a special urea decomposition catalyst. The second reaction step, i.e. the catalytic hydrolysis of HNCO was studied on the anatase TiO2(101) surface and Al2O3(100) surface with ab initio density functional theory (DFT) calculations using a cluster model as well as with in situ diffuse reflectance infrared Fourier transform spectra (DRIFTS) investigations and kinetic experiments. The following mechanistic pathway has been identified to be most feasible: HNCO dissociatively adsorbs on the metal oxide surface as isocyanates, which are attacked by water, thereby forming carbamic acid at the surface. In a further step this intermediate is transformed to a carbamate complex, which leads to CO2desorption and consequently NH3formation. The comparison between the sum of the theoretical vibrational spectra of the reaction intermediates with the in situ DRIFT spectra also strongly supports the accuracy of the second reaction pathway. This mechanism holds also for the HNCO hydrolysis over c-Al2O3and the reactivity compared to TiO2was found to be consistent with the heights of the barriers in the energy diagrams. Based on these promising preliminary results a computational screening has been started in order to predict the most active metal oxides and surfaces for this reaction.
Keywords Titanium dioxide TiO2(101) surface Aluminium oxide c-Al2O3(100) DFT DRIFTS Cluster model Isocyanic acid Carbamic acid Carbamate group
The selective catalytic reduction (SCR) process with urea is an efficient technology for the reduction of nitrogen oxides emissions of diesel vehicles [1–4]. The reason for the use of urea is its easy thermal decomposition to ammonia, which is the real reducing agent in the SCR reaction. In a typical SCR system urea thermolyses in the hot exhaust gas to ammonia and isocyanic acid (HNCO), which hydrolyzes on the SCR catalyst to ammonia and carbon dioxide [2,5–18]. The SCR catalyst can be disburdened from this additional reaction by the application of a specialized hydrolysis cat-alysts upstream of the SCR catalyst [2,5,6]. We screened a series of single and mixed metal oxides for this reaction and titania in the anatase modification was found to be a most active . Compared to titania, alumina proved to be much less active and silica showed only low activity for the HNCO hydrolysis. In order to explain the superior proper-ties of titania for this reaction we investigated the mecha-nism of the HNCO hydrolysis on the TiO2 anatase (101) surface by a combination of DFT calculations and experi-mental techniques [20,21]. Two reaction pathways could be identified, a first in which water enters the reaction sequence at a late stage and which proceeds via molecular adsorption of HNCO and oxygen vacancy formation , and a second in which water is involved right from the beginning and which proceeds by dissociative adsorption of HNCO and carbamic acid formation . The second reaction scheme with an early participation of water is more likely than our
I. Czekaj (&) O. Kro¨cher
Department General Energy, Paul Scherrer Institute, 5232 Villigen PSI, Switzerland
e-mail: email@example.com DOI 10.1007/s11244-009-9344-8
first reaction scheme since it involves lower energy barriers. Moreover, the measured reaction orders of the HNCO hydrolysis over TiO2 and the measured in situ DRIFT spectra could only be reconciled with the second reaction pathway.
The scope of the present work was to extend our theo-retical study on the hydrolysis of HNCO over titania to other metal oxide catalysts. We chose c-Al2O3 as second candidate since it was found to be also quite active for the HNCO hydrolysis  and since it plays an important role in other NOxreduction processes as well . Numerous theoretical studies about pure and modified c-Al2O3 sys-tems were performed previously [23–25] using both peri-odic and cluster models. Other reasons for our selection of c-Al2O3were that it is a single metal oxide and that a similar HNCO hydrolysis mechanism can be assumed on this rather simple material. Although it is reasonable to assume that this relatively simple reaction proceeds via the same mechanism over different metal oxides, this assumption has to be carefully checked for every new material. In our study, the hydrolysis of HNCO on Al2O3(100) was compared with that on TiO2(101) by modeling the Os-Ms unit of both materials with large molecular clusters using the density functional theory. This comparative study is a first step towards our goal to establish a virtual screening of catalysts for this reaction, which can provide energy barriers, acti-vation energies and activities of different catalysts without the influence of the preparation method. The activity of real catalysts is determined by the share of the different modi-fications in the bulk and the share of the exposed surfaces as well as by the surface area, pores size distribution and other factors, such as impurities.
The tetragonal anatase phase of titanium dioxide, TiO2, was chosen for our investigations (see details in ). The
TiO2anatase (101) surface is shown in Fig.1a, where the different titanium and oxygen sites are highlighted.
The cubic phase [26, 27] of defective alumina spinel, Al2O3,is described by the space group Fd-3m with lattice constants a = b = c = 7.911 A˚ . The crystal unit cell of defective alumina spinel contains 56 atoms, where Al occupies two different types of positions—8a, 16d, and oxygen 32e sites.
Inside the bulk both AlO6octahedra and AlO4tetrahedra are present with Al–O distances equal to 1.94 and 1.78 A˚ , respectively. The bulk is built by six- and four-fold coor-dinated aluminium and three- and four-fold coorcoor-dinated oxygen. Figure 1c shows the structure of the c-Al2O3(100) surface. Two different aluminium sites with four- and five-fold coordinated aluminium, AlO4and AlO5, as well as two different three-fold coordinated oxygen sites, O(3) and O0(3), can be distinguished. It is important to note that Al(4) is always located below the Al(5) centres and that the rows of AlO5pyramids are separated from each others by rows of AlO4tetrahedra.
Two surface planes are predominantly detected in the diffraction patterns of c-Al2O3, namely the (110) and (100) surfaces. Following some previous studies of alumina by Handzlik et al. , the (100) surface was chosen for our studies. Three different distances are observed between the aluminium atoms on the (100) surface of alumina: (i) 3.28 A˚ between Al(4)–Al(5) atoms, (ii) 2.79 A˚ between Al(5)–Al(5) atoms in the AlO5 row and (iii) 5.59 A˚ between Al(4)–Al(4) atoms. The surface exhibits specific holes with a distance of 2.90 and 2.79 A˚ between the O(3) atoms. The adsorbates have good access to the electrophilic M(5) centers, which are, therefore, preferably covered by HNCO and H2O.
In our studies the catalyst surfaces were modeled by clusters of different size and geometry, which were satu-rated by hydrogen atoms with ROH= 0.97 A˚ . For modeling of the TiO2(101) surface, the clusters Ti2O9H10, Ti8O28H24, Ti13O43H34 and Ti15O50H40 were selected , among which the Ti8O28H24cluster proved to be best suited for the further reaction studies (Fig. 1b). In case of c-Al2O3, the
Fig. 1 Characteristic surface sites at a TiO2anatase (101) and c Al2O3(100) and the corresponding model clusters bTi8O28H24and d Al11O30H27
clusters Al11O30H27, Al15O40H35 and Al25O58H41 were checked, from which Al11O30H27 was finally selected for this study (Fig.1d).
The electronic structure of clusters and of all reaction intermediates was calculated by ab initio density functional theory (DFT) methods (StoBe code ) using the gen-eralized gradient corrected functional (RPBE) [29,30] and linear combinations of atomic orbitals [31,32]. A double zeta valence polarization (DZVP) type was used for the orbital basis sets of Ti (63321/531/41), Al (6321/521/1), O, C, N (621/41/1), and H (41). Auxiliary basis sets, such as (5,5;5,5) for Ti, (5,4;5,4) for Al, (4,3:4,3) for O, C, N, and (41) for H, were applied to fit the electron density and the exchange-correlation potential. A detailed analysis of the electronic structure of the clusters was carried out using Mulliken populations  and Mayer bond order indices [34,35]. In the calculations for all reaction steps, the low spin states were found to be energetically favorable.
The adsorption energies of the adsorbates on the MxOyHzcluster were calculated as follows:
Eadðadsorbate=catalystÞ ¼ Etot adsorbate=MxOyHz Etot MxOyHz
where Etot(adsorbate/MxOyHz) is the total energy of the adsorbate/catalyst surface complex, Etot(MxOyHz) and Etot(adsorbate) are the total energies of pure MxOyHzand the adsorbate, respectively.
The calculations of the vibrational frequencies were performed with harmonic approximations as well as an anharmonicity fit in the Morse potential function, as implemented into StoBe code . Theoretical vibrational spectra were obtained by convolution of the vibrational spectra of the individual adsorbates, applying Gaussian line-shapes. The frequencies are reported as obtained from the calculations, without scaling.
Powdered TiO2in the anatase modification was used in the experimental investigations (SBET = 57 m
/g). Isocyanic acid was produced by thermal decomposition of cyanuric acid and subsequently mixed with the feed gas, as descri-bed in .
A Thermo Nicolet Nexus 860 FT-IR spectrometer was used to for the in situ measurement of diffuse reflectance infrared Fourier transform spectra (DRIFTS). The catalyst sample was purged in situ for 1 h at 450°C with a flow of N2gas. The studies of HNCO adsorption were performed at various temperatures up to 450°C. At each temperature the catalyst was first been treated with &70 ppm of HNCO in N2for 15 min and then exposed to a N2flow for 15 min in order to remove physisorbed adsorbates from the surface.
Finally, water pulses were added through a capillary to start the hydrolysis reaction.
3 Results and Discussion
The calculations revealed that dissociative as well as molecular adsorption of HNCO is possible and energeti-cally feasible on both the TiO2(101)  and the Al2O3(100) surface [37,38]. Figure2shows the geometric and electronic structures of HNCO and the interacting sites of TiO2(101) and Al2O3(100), represented by the Ti8O28H24 (see Fig.1b) and the Al11O30H27 cluster (see Fig. 1d). Information about adsorption energy, atomic charges (Mulliken analysis), distances (A˚ ) and bond orders (Mayer bond analysis) are also included in Table 1.
For investigation of the reaction mechanism of the HNCO hydrolysis the co-adsorption of HNCO and H2O at the catalyst surface had to be considered, which comprises the competitive adsorption of water and HNCO and the interaction of water from the gas phase with HNCO adsorbates. This requires the presence of free neighbored five-fold coordinated metal sites.
Figure3shows a comparison of the energy levels for the intermediates observed during hydrolysis of HNCO. Adsorption of HNCO is actually possible in the presence of water, because the dissociative adsorption of HNCO is energetically competitive to the dissociative adsorption of water on the TiO2and Al2O3surface. The –NCO group is stabilized at a M(5) center with an adsorption energy of
Fig. 2 a, b Molecular and c, d dissociative HNCO adsorption at a, c TiO2(101) and b, d c-Al2O3(100)
-0.91 and -1.11 eV (see Fig.3b) for TiO2 and Al2O3, respectively, whereas water adsorbs dissociatively with an adsorption energy of Ead= -0.84 and -1.06 eV (see Table1). Although molecular adsorption of water should be energetically even more favored (Ead= -1.19/-1.52 eV), dissociative adsorption of water is observed over the whole
temperature range and even at very low temperatures (50°C) .
The –NCO groups at the catalyst surface are attacked by a water molecule from the gas phase and a carbamic acid complex is immediately formed (–NHCOOH). As shown in Fig.3c, the carbamic acid is bound to the M(5) atoms with
Table 1 The HNCO adsorption at TiO2(101) and c-Al2O3(100)
TiO2 Al2O3 (a) Molecular EB(HNCO) (eV) -0.40 -0.72 EB(H2O) (eV) -1.19 -1.52 N–M b.o. (b.d. [A˚ ]) 0.20 (2.43) 0.18 (2.26) N–C b.o. (b.d. [A˚ ]) 1.95 (1.24) 1.84 (1.25) (b) Dissociative EB(HNCO) (eV) -0.91 -1.11 EB(H2O) (eV) -0.84 -1.06 N–M b.o. (b.d. [A˚ ]) 0.59 (1.99) 0.68 (1.94) N–C b.o. (b.d. [A˚ ]) 2.23 (1.21) 2.16 (1.21) (c) Calculated vibrational frequencies (cm-1) of individual surface intermediates
Sym. Asym. Sym. Asym. m (NCO) HNCO 1279 2266 1263 2264 NCOaq 1351 2194 1342 2274 NCO 1345 2181 1364 2293 m (N–H/H–N–H) NHCOOH 3462 – 3280 – NH2CO2 3346 3482 3364 3488 NH2aq 2905/3349 3466 3406/3425 3533 NH3aq 2955/3381 3492 3068/3394 3484
Fig. 3 The energy diagram for the hydrolysis of HNCO on TiO2(101) (blue levels) and c-Al2O3(100) (red levels): aCluster ? HNCO reference level. b Dissociative adsorption of HNCO on the catalyst. cWater attack on the NCO group at the M(5) site and formation of surface carbamic acid (NHCOOH). d Transfer of the carboxyl H to the NH group. eFormation of adsorbed carbamate (NH2CO2) at the M(5) site. f CO2separation from the NH2surface group. g CO2 desorption and stabilization of the NH2group at M(5). h Migration of the H from adsorbed water to NH2. i NH3 at the M(5) site
an adsorption energy of -2.13 eV (TiO2) and -2.56 eV (Al2O3). By a change of the conformation of the carbamic acid, in which the hydrogen atom at the oxygen is inter-nally transferred to the nitrogen, a carbamate complex (–NH2CO2) can be formed at the surface (Fig.3e). This process requires a high energy of about 2.14 eV for TiO2 and 3.79 eV for Al2O3 (Fig.3d) with respect to the car-bamic acid level (Fig.3c). As a matter of fact, the high energy needed for the internal hydrogen transfer from the carboxylate group in –NHCOOH to the nitrogen in H2NCOO could be overcome in the real system by dehy-drogenation of carboxylate group to another molecule (e.g. water) and hydrogenation of the –NH group from an external hydrogen source. The important fact is that the formation of the carbamate complex from carbamic acid (Fig.4c–e) is exothermic for TiO2(-0.16 eV) and slightly endothermic for Al2O3(0.07 eV). The carbamate complex decarboxylates (Fig.3g) and the NH2group remains at the M(5) atom. The hydrogen missing for the formation of ammonia can be obtained from a water molecule adsorbed at a neighboring M(5) atom. The hydrogen transfer from a second water molecule is facilitated by the very low energy level of the system after the adsorption of water (-3.56 eV for TiO2 and -3.02 eV for Al2O3; Fig.3h). The NH3, formed by the reaction of NH2groups with adsorbed water molecules, is finally released from the catalyst surface, which enriches the catalyst surface with OH groups. This is in agreement with the in situ DRIFTS experiments descri-bed below, since strong OH/water vibrations are always visible after reaction.
The comparison between the theoretical vibrational spectra of the reaction intermediates of the HNCO adsorp-tion on TiO2and Al2O3with the in situ DRIFT spectrum for TiO2 is shown at Fig.4. The theoretical spectra were obtained by summation of the spectra of the individual adsorbates such as ammonia, carbamic acid and HNCO as well as amino, carbamate, and isocyanate groups, each influenced by an aqueous environment in form of H2O or OH groups.
Exposure of the catalyst to HNCO at 150 °C resulted in the evolution of a strong band at 2209 cm-1together with less intense bands in the range 3524–3163 and 1619– 1190 cm-1(see upper spectrum in Fig. 4). Some of vibra-tions calculated theoretically are listed in Table1c. The strong band at 2209 cm-1 is assigned to the asymmetric stretching vibrations of –NCO groups adsorbed at the sur-face. From our theoretical studies we found that the main contributions to these vibrations come from dissociatively adsorbed HNCO stabilized by M(5) centers evoking the vibration at 2234 cm-1in the neighborhood of strong OH groups and the vibration at 2181 cm-1 in the absence of OH groups. However, small amounts of weakly adsorbed HNCO in molecular form can be found at 2266 cm-1, which is very close to the vibration of gaseous HNCO. Our theoretically predicted vibrations on TiO2 are consistent with results of Hauck et al. , where this band has components at 2189, 2230 and 2255 cm-1. In the case of the Al2O3catalyst the theoretically predicted vibrations of the –NCO groups are at 2274 cm-1in case of dissociative adsorption and at 2264 cm-1 in case of molecularly adsorbed HNCO. These vibrations are also in good agree-ment with experiagree-mental data presented recently by Ozensoy et al. , who recorded TD-FTIR spectra at 120°C and who found bands at 2143 and 2254 cm-1. The calculated vibrations of NCOaq and HNCO are very close to each other, which suggests that on Al2O3 more HNCO can be found in molecular form. This is in good agreement with the higher adsorption energy of molecular HNCO on Al2O3 (-0.72 eV) compared to TiO2(-0.40 eV) (Table1a).
The theoretical bands below 1800 cm-1 and above 3000 cm-1in Fig.4have a similar shape as in the experi-mental TiO2spectrum, but they are slightly shifted to higher frequencies. The lower-frequency bands (1200–1800 cm-1) in the calculated spectrum in Fig.4 correspond to the bending vibrations of NH2or NH3as well as NH2CO2and NHCOOH and the symmetric stretching vibrations of NCO influenced by water. The high-frequency bands (3000– 3500 cm-1) are the sum of the N–H stretching vibrations of the individual adsorbates (see Table1c) influenced by water. The intermediate complexes, such as –NCO or carbamic acid, have stronger stabilisation energies at the Al2O3 surface, which simply means that it will be more difficult to convert them into the following surface complexes. This 1000 1400 1800 2200 2600 3000 3400 3800 Wavenumber [cm-1] Absorbance [a.u.] TiO2-DRIFT TiO2-DZVP Al2O3-DZVP
Fig. 4 Theoretical vibrational IR spectra and experimental DRIFT spectra of TiO2 after HNCO adsorption (70 ppm) at 150°C for 15 min followed by purging with nitrogen for 15 min as well as theoretical vibrational IR spectra of Al2O3after HNCO adsorption
result is in agreement with our experimental result that Al2O3 has a lower activity than TiO2 for the HNCO hydrolysis (Fig.5).
DFT calculations show that the hydrolysis of HNCO is possible over both TiO2and Al2O3catalysts and proceeds along similar reaction paths. The course of the reaction can be summarized as follows: water attacks the –NCO group and a carbamic acid complex is formed at the surface in an exothermic reaction without an energy barrier. Then, the carbamic acid is transformed into a carbamate complex, which leads to CO2desorption and the formation of an NH2 group. In the last step of the hydrolysis reaction, NH3 is formed via hydrogen transfer from an OH group or from molecularly adsorbed water, the latter being energetically favored. It is important to note that the reaction occurs with a lower energy barriers on the TiO2(101) than on the Al2O3(100) surface. Two conditions for HNCO hydrolysis catalysts are the existence of free M(5) sites and surface reactivity with water. There is a large population of M(5) sites at the surface of both catalysts, but they differently interact with water and HNCO, i.e. reaction intermediates, such as water, NCO species, carbamic intermediates and NHx species are bound with unequal strength. The inter-mediates are much stronger bound to the alumina surface which leads to higher reaction barriers and makes alumina unfavorable for HNCO hydrolysis, in accordance with the experimentally found order of activities.
Acknowledgement The calculations were done partially using the unix farm and the linux farm at the Paul Scherrer Institute as well as at the Swiss National Supercomputing Centre.
1. Piazzesi G, Kro¨cher O, Elsener M, Wokaun A (2006) Appl Catal B 65:55
2. Kleemann M, Elsener M, Koebel M, Wokaun A (2000) Ind Eng Chem Res 39:4120
3. Belson DJ, Strachan AN (1982) Chem Soc Rev 11:41
4. Koebel M, Elsener M, Marti T (1996) Combust Sci Technol 121:85
5. Busca G, Lietti L, Ramis G, Berti F (1998) Appl Catal B 18:1 6. Piazzesi G, Nicosia D, Devadas M, Kro¨cher O, Elsener M,
Wokaun A (2007) Catal Lett 115:33
7. Beltran A, Sambrano JR, Calatayud M, Sensato FR, Andres J (2001) Surf Sci 490:116
8. Hadjiivanov K, Klissurski DG (1996) Chem Soc Rev 25:61 9. Tsyganenko AA, Filimonov VN (1972) Spectrosc Lett 5:477 10. Ramis G, Busca G, Lorenzelli V, Forzatti P (1990) Appl Catal
11. Ramis G, Busca G, Lorenzelli V (1987) J Chem Soc Faraday Trans I 83:1591
12. Fernandez A, Leyrer J, Gonzales-Elipe AR, Munuera G, Knoz-inger H (1988) J Catal 112:489
13. Busca G, Saussey H, Saur O, Lavalley J, Lorenzelli V (1995) Appl Catal 14:245
14. Bredow T, Jug K (1995) Surf Sci 327:398 15. Solymosi F, Rasko J (1980) J Catal 65:235 16. Solymosi F, Bansagi T (1979) J Phys Chem 83:552
17. Branda MM, Belelli PG, Ferullo RM, Castellani NJ (2003) Catal Today 85:153
18. Gao H, He H (2005) Spectrochim Acta A 61:1233
19. Piazzesi G (2006) The catalytic hydrolysis of isocyanic acid (HNCO) in the urea-SCR process, PhD thesis, Diss. ETH No. 16693, Zurich
20. Czekaj I, Piazzesi G, Kro¨cher O, Wokaun A (2006) Surf Sci 600:5158
21. Czekaj I, Kro¨cher O, Piazzesi G (2008) J Mol Catal A 280:68–80 22. Ozensoy E, Herling D, Szanyi J (2008) Catal Today 136:46 23. Handzlik J, Ogonowski J, Tokarz-Sobieraj R (2005) Catal Today
24. Digne M, Sautet P, Raybaud P, Euzen P, Toulhoat H (2004) J Catal 226:54–68
25. Ionescu A, Allouche A, Aycard JP, Rajzmann M, Hutschka F (2002) J Phys Chem B 106:9359–9366
26. Zhou R-S, Snyder RL (1991) Acta Crystallogr B 47:617–630 27. Verwey EJW (1935) Z Kristallographica 91:317–320
28. The program package StoBe is a modified version of the DFT-LCGTO program package DeMon, originally developed by A. St.-Amant and D. Salahub (University of Montreal), with extensions by Pettersson LGM and Hermann K
29. Perdew JP, Burke K, Ernzerhof M (1996) Phys Rev Lett 77:3865 30. Hammer B, Hansen LB, Norskov JK (1999) Phys Rev B 59:7413 31. Labanowski JK, Anzelm JW (eds) (1991) Density functional
methods in chemistry. Springer, New York
32. Godbout N, Salahub DR, Andzelm J, Wimmer E (1992) Can J Phys 70:560
33. Mulliken RS (1955) J Chem Phys 23: 1833, 1841, 2388, 2343 34. Mayer I (1983) Chem Phys Lett 97:270
35. Mayer I (1987) J Mol Struct Theochem 149:81
36. Friedrich C (2004) Geometrische, elektronische und vibronische Eigenschaften der reinen und defektbehafteten V2O5 (010)-Obe-rfla¨che und deren Wechselwirkung mit Adsorbaten: Theoretische Untersuchungen, FU Berlin
37. Cant NW, Chambers DC, Liu IOY (2003) Appl Catal B 46:551 38. Hauck P, Jentys A, Lercher JA (2007) Catal Today 127:165–175
0 10 20 30 40 50 60 70 80 90 100 0 100 200 300 400 T [°C] YNH3 [%] TiO2 γ-Al2O3
Fig. 5 Catalytic activity of a TiO2(anatase) and b c-Al2O3in the HNCO hydrolysis. Wcat.= 150 mg, gas flow rate = 200 LN/h, inlet flow composition = 1000 ppm HNCO, 5% H2O, 10% O2 and N2 balance